Embed Size (px)
Transcript of Amirkhanian Nanocomposite
Preparation and rheological characterization of asphalt binders reinforced with layered silicate nanoparticlesAbolfazl Zare-Shahabadi * , Ali Shokuhfar, Salman Ebrahimi-NejadAdvanced Materials and Nanotechnology Research Lab, Faculty of Mechanical Engineering, K.N. Toosi University of Technology, Postal Code: 19991-43344, Tehran, Iran.
Abstract Bentonite clay (BT) and organically modified bentonite (OBT) were used to reinforce and modify a bituminous paving asphalt binder. The modified asphalt binders were produced by melt processing under sonication and shearing stresses. The interlayer spacing of silicate layers in bentonite, organically modified bentonite and the modified asphalt binders were analyzed by wide angle X-ray diffraction (WAXD). The softening point, viscosity and ductility of the modified asphalts were tested as a function of clay content and clay type. The dynamic shear rheological tests showed that the modified asphalts have higher rutting resistance. Bending beam rheometer (BBR) test results for aged specimens (through rolling thin film oven (RTFO) and pressure aging vessel (PAV)) indicated that adding BT and OBT can significantly improve low temperature rheological properties and cracking of asphalt. Keywords: Asphalt binder; Bentonite; Layered Silicates; Nanocomposites.
1. Introduction Asphalt (or bitumen) is used in road pavements as the binder of aggregates in a great extent all around the world. Asphalt pavements must undergo heavy loads and unfavorable environmental conditions for an acceptable period of time. Hightemperature rutting and low temperature cracking are the most considerable limitations of unmodified and pure asphalts . Therefore, modification and reinforcement of asphalt binder is necessary. Asphalt usually is a byproduct of crude oil refining process in petroleum refineries, and it is a complex heterogeneous mixture of hydrocarbons . The first studies on the use of nanoclay or layered silicate nanoparticles as filler and reinforcing agent were reported by Toyotas researchers with the production of nylon 6/clay Nanocomposites [3,4]. Polymer/layered silicate nanocomposites have showed significantly enhanced mechanical , thermal  and barrier  properties compared to the pure polymer matrix with addition of a minimal amount of filler. Therefore, various types of polymers (such as addition polymers [8-10], condensation polymers [11-13] and biodegradable polymers [14, 15]) have been studied and used as the matrix in these nanocomposites.
-Corresponding author. Tel: +98 2184063304 Fax:+98 3518210670 Email addresses: email@example.com , firstname.lastname@example.org (A. Zare-Shahabadi) , email@example.com (A. Shokuhfar), firstname.lastname@example.org (S. Ebrahimi-Nejad)
The dispersion of clay particles in the matrix can form three types of structures (Fig. 1). The first one is the conventional composites structure in which the silicate platelets are agglomerated. The second one is intercalated nanocomposites structure, where some matrix molecules are inserted between individual silicate layers, but the layers remain parallel. The third type is the exfoliated nanocomposites structure, in which the layered structure of the clay is disrupted, with the silicate layers no longer close enough to interact with each other and nanometric particles are fully dispersed in the matrix . Typical clays capable of forming intercalated or exfoliated structures include montmorillonite, flurohectorite and bentonite . In order to obtain a good interfacial adhesion and mechanical properties, the hydrophilic clay needs to be modified prior to introduction in most polymeric matrices that are organophilic. Clay modification is generally achieved by ion exchange reactions of organophilic cations by sodium ions which are naturally between the clay layers . Clay-containing nanocomposites may be obtained mainly by three methods: in-situ polymerization [19-21], solution blending [22-24] and melt processing [25-27]. Yu and coworkers  have used montmorillonite (MMT) clay and organically modified montmorillonite (OMMT) to modify asphalt. They have investigated the physical properties, dynamic rheological behaviors and the high temperature storage stability of the modified asphalts. They showed that the MMT and OMMT modified asphalts have higher rutting resistance and very good storage stability. Also, in a recent work, the effect of OMMT on thermo-oxidative and UV aging properties of asphalt is investigated by Yu et al . In this paper, sodium bentonite (BT) and organically modified sodium bentonite (OBT) are used to reinforce and modify asphalt binder. BT is a sedimentary rock consisting, to a large proportion, of clay minerals with a typical 2:1 layered structure (smectites) and a high concentration in sodium ions . Indeed, BT is a clay mineral which is rich in MMT . BT has natural abundance and low cost which can make it economically more suitable for this purpose. In this research the physical properties and high temperature dynamic rheological behavior of the BT and OBT modified asphalt binders were studied. Also, low temperature cracking properties of the modified asphalt binders were evaluated after artificially short-term and long-term aging. 2. Experimental Methods 2.1. Materials Asphalt, 60/70 penetration grade bituminous paving asphalt binder was produced in Tehran refinery and supplied by Pasargad Oil Co, Tehran, Iran. The physical properties of the asphalt are listed in Table 1, and its chemical compositions are listed in Table 2. Sodium bentonite clay with cation exchange capacity (CEC) of 110 meq/100 g was supplied by Chavosh Maadan Co, Tehran, Iran. Octadecylamin and HCl were purchased from Merck Co, Germany. 2.2. Clay modification Before the clay modification, a purification process was performed. The purification process consisted of the following steps: (a) water dispersion of the as received clay and 24 h aging to ensure swelling of clay, (b) elimination of supernatant and sediments. The organically modified bentonite was produced by ion exchange reaction between bentonite and octadecylammonium salt which was obtained after protonation of octadecylamine by adding hydrochloric acid to the reaction medium during the process, before the ion exchange reaction can occur. Thus, octadecylamine was previously
mixed with HCl in water and heated at 80o C for a few minutes. The CEC ratio of ODA/clay was 1.5 and the molar ratio of ODA/HCl was 1:1. The as-protonated surfactant was drop wise added to the clay suspension and maintained at 80o C for 1 h under vigorous stirring. Then the suspension was cooled to room temperature. This suspension was dispersed and washed with water twice. A third dispersion and washing was accomplished using a 50/50 ethanol/water mixture. The final washed modified clay was dried at 75o C by a hot air blower device, and then powdered by a ball mill device. The organically modified bentonite powder was sieved through a 50 m steel mesh. This method is similar to the method described in reference . However, in this work the solid percent of the clays that is modified during the process has been varied (10% and 20%) and a different clay drying procedure has been used. 2.3. Preparation of modified asphalts The modified asphalts were prepared at 160 oC. The measured amounts (1, 2, 4, 5, 6 wt%) of BT or OBT were gradually added into 1.5 liter volumes of the base asphalt binder when mixing by a simple mixer in beakers. The mixtures were blended at 4000 rpm rotational speed for about 1 hr using a Silverson-L4RT high shear mixer, and then sonicated with a Missonix sonicator device with 20kHz sound waves for 10 minutes in order to allow the better dispersion of BT or OBT nanoparticles. 2.4. Aging of asphalt binders Asphalt binders age mainly due to two different mechanisms: (a) volatilization of light oils present in the asphalt, (b) oxidation by reacting with the oxygen in the environment. The blending and agitation in the hot mixing facility and during placement ages the binder by both mechanisms because of the high temperature and air flow involved in the process. The rolling thin film oven (RTFO) procedure is used to simulate this form of aging. After the asphalt pavement is constructed, aging continues, but the oxidation mechanism dominates because of the relatively moderate temperatures of the environment. The pressure aging vessel (PAV) is used to simulate this in-service aging . The base asphalt binder, 5% BT modified asphalt and 5% OBT modified asphalt were artificially short-term and then long-term aged through RTFO aging (ASTM D 2872) and then PAV aging (AASHTO PP1). The aged samples were used in the bending beam rheometer test. 2.5. Characterizations Wide angle X-ray diffraction (WAXD) of the clays and modified asphalts was performed in a Brucker axs-D8 diffractometer using CuK radiation ( = 0.154 nm; 40 kV, 30 mA) in order to evaluate the evolution of clay d 001 reflections. The scanned range was from 1 to 12 in the 2 with a scanning rate of 1.2 min1. The physical properties of the asphalts, including softening point (Strassentest ring and ball Instrument), ductility at 25oC (Strassentest Instrument) and viscosity at 135oC (Bohlin Instrument), were tested according to ASTM D 36, ASTM D 113 and ASTM D 4402, respectively. Each of these tests were performed 3 times for the (0, 1, 2, 4, 6 wt %) BT and OBT modified asphalts and the average values of the results were used. A Dynamic Shear Rheometer (Bohlin Instrument) was used for dynamic rheological measurements in plateplate mode (1mm thickness, 25 mm diameter) for base asphalt, 5% BT modified asphalt and 5% OBT modified asphalt according to AASHTO TP5. Temperature sweeps from 46 to 70oC with 6oC increments were applied at a fixed frequency of 10 rad/s and variable strain.